Polyvinyl alcohol/soy protein isolate nanofibrous patch for wound-healing applications
- 215 Downloads
Soy protein isolate (SPI), due to its biocompatibility, biodegradability, abundance and being inexpensive, is a suitable polymer for medical applications. In this study, electrospun nanofibrous mats (ENMs) and casting films (CFs), comprising polyvinyl alcohol (PVA)/SPI, were prepared and compared. Both crosslinked ENMs and CFs physical, chemical, mechanical, and biological properties were investigated for wound-healing applications. Considering the importance of exudate absorption by wound dressing the uptake test of all samples was performed in simulated exudate solution. The amount of absorbed exudate, water vapor transmission rate, and mechanical elongation for CFs were 69.243% ± 22.7, 266.7 g/m2 day, and 2.0825% and increased to 383.33% ± 105.3, 1332.02 g/m2 day, and 12.292% in the case of ENMs, respectively. There was no significant difference between cell supporting of the two samples due to similar composition and their non-toxic properties. The results showed that ENMs have promising potential in wound-healing applications.
KeywordsSoy protein isolate Electrospun nanofibrous mat Wound healing
In recent years, there is a growing interest in using naturally derived biomaterials to reduce the use of petrochemical feedstock and manufacture high-quality, cost-effective, biodegradable, and biocompatible products. From this aspect, these materials from renewable resources will be an eco-friendly substitute for petroleum-based materials (Koshy et al. 2015). Merits including bioactivity, biodegradation, and presence of natural binding sites for manipulating the cell adhesion and growth both in vitro and in vivo have made animal- and plant-based proteins ideal biomaterials (Chien et al. 2013). Soybean is widely available in the world and is considered as a cost competitive feed stock polymer. There are three forms of commercial soy protein based on the extraction process and each has different protein content; defatted soy flour, soy protein concentrate, and soy protein isolate (SPI) containing approximately 53%, 74%, and 93% protein, respectively. All these soy products are representatives of biodegradable ‘‘green’’ composites due to their good performance (Cho et al. 2010).
Through the production of oil, the obtained product from defatted soy flakes is SPI which is the purest form of the protein and has a minimum of 90% protein content. Due to its abundance, biodegradability, biocompatibility, and being inexpensive, SPI is a suitable polymer for medical applications (Shankar et al. 2013). Amino acids of aspartic acid (aspargine) and glutamic acid (glutamine), non-polar amino acids (glycine, alanine, valine, and leucine), basic amino acids (lysine and arginine), and less than 1% of cysteine are presented in the chemical structure of the soy protein also make an advantage for biomedical application of SPI. Soy protein can be modified through chemical, physical, and enzymatic modifications for a variety of biomedical applications due to the presence of high amounts of reactive groups, such as –NH2, –OH, and –SH. Having a greater storage stability in comparison with other biodegradable polymers and natural proteins, as well as being of non-animal origin (plant derived), are additional advantages of soy protein for biomedical applications (Ramji and Shah 2014). SPI-based products are formed through denaturation of the protein structure from native state and reformation of new configurations through new linkages within the protein molecule. Changes in pH, electrical force, mechanical force, or heat are the possible ways that denaturation can be induced (Koshy et al. 2015).
Polyvinyl alcohol (PVA) is a synthetic polymer that has features such as being semi-crystalline, water soluble, biodegradable, and biocompatible with human tissues. This polymer is produced in the largest quantity worldwide (Taghizadeh and Sabouri 2013). Contact lenses, drug delivery devices, wound dressings, orthopedic devices, and artificial organs are some examples of PVA used in various pharmaceutical and biomedical applications. It can be crosslinked by chemical agents such as glutaraldehyde (GA), acetaldehyde, and formaldehyde (Ye et al. 2014). To fabricate biodegradable composites, PVA can be combined with natural polymers. This blended PVA/natural polymer has a couple of advantages SUCH AS biodegradability, biocompatibility, chemical resistance, and excellent physical properties which makes it a promising biomaterial in many fields of industrial applications (Su et al. 2010a, b).
An ideal wound dressing should possess some characteristics such as non-toxicity, biocompatibility, easy application, appropriate water vapor permeability, and optimal water uptake. A minimum adherence to the wound bed which provides an easy removal of the wound dress, so it would not cause a secondary trauma to the regenerated skin. Furthermore, a suitable microenvironment is necessary that a wound dressing should provide for wound healing (Saeed et al. 2017; Doulabi et al. 2015). Depending on the injury location and the type of the exudates, the mechanical and physiochemical properties of the wound dressing should suit the condition with adjustments (Moghadas et al. 2016). In this aspect, blend polymers are more beneficial in providing more previously mentioned requirements in comparison with a single polymer, since their properties are improved (Doulabi et al. 2015).
Recently, electrospinning with capability to form polymeric fibers, of different diameters, has gained attention as fabrication technique for preparation of fibrous biomaterial. The morphological resemblance to native extracellular matrix (ECM), high surface/volume ratio, high porosity, and pore interconnectivity is amongst the main features of electrospun structures (Khorshidi et al. 2016a, b).
Previous studies showed that the compatibility of the PVA/SPI blend could be enhanced by the presence of glycerol and/or greater modification of the interfacial adhesion (Su et al. 2010a, b). However, these blends are unstable in contact with aqueous media. To prevent the dissolution of these blends in aqueous media and considerable loss of mechanical strength, crosslinking procedures are necessary (Khorshidi et al. 2016a, b).
The aim of this study is the fabrication and evaluation of films and nanofibers based on polyvinyl alcohol/soy protein isolate using solvent-casting and electrospinning methods for the purpose of wound healing. Different studies of blending these two polymers have been carried out either in the form of electrospinning (Cho et al. 2010; Zhang et al. 2003) or film formation (Su et al. 2008), but to the best of our knowledge, no work in the literature has been reported the composition of PVA/SPI/glycerol for the purpose of wound healing.
Materials and methods
PVA (Mw 72000 g mol−1, the degree of hydrolysis ≥ 98%) was purchased from Merck. Food grade SPI powder (batch no: E24) containing ≥ 90% protein and ≤ 7.0% moisture was purchased from FOODCHEM. Analytical grade glycerol (Mw 92.09) with ≥ 99% purity was purchased from MP Biomedicals. Laboratory grade nonionic surfactant Triton X-100 (t-Oct-C6H4-(OCH2CH2)xOH x = 9–10) was purchased from Sigma. Analytical grade sodium hydroxide (NaOH) pellets were used to prepare a 1 M solution at room temperature. Dialdehyde-crosslinking agent of glutaraldehyde (25 wt% in H2O) was purchased from Merck. Laboratory grade acetone with ˃ 99% purity and hydrochloric acid with ≥ 37% purity was purchased from Ghatran ShimiT.Co.IRAN.
Films of PVA/SPI/glycerol were formed using the solvent-casting method. PVA aqueous solution (10 wt%) was prepared by dissolving PVA in deionized water in a water bath at 70 °C for 2 h. SPI aqueous solution (8.5 wt%) was prepared by stirring in deionized water at room temperature for 10–15 min. To form SPI-based films, the protein structure needs to be denatured. Here, the denaturation of SPI induced by altering the pH by adding 1 M NaOH to the solution and applying heat. Therefore, SPI solution was stir-heated in a water bath at 80 °C for 30 min with the adjusted pH (7.88 ± 0.12). These two solutions were mixed with a mass ratio of 50:50, and to acquire a uniform solution, it was stirred in a water bath at 70 °C for 1 h. The amount of 5 wt% of the plasticizer (glycerol) was added into the final solution. To obtain the equal thickness, 5 mL of solutions were poured into 8 mm diameter polystyrene petri dishes and cooled to room temperature to remove bubbles. Finally, aqueous resins were oven dried at 50 °C for 6 h (Su et al. 2010a, b).
Solution preparation for the process of electrospinning was carried out precisely the same as the preparation of the solution for CFs with the same amount of polymers. To have a spinnable solution, denaturation of the native state of the protein has to occur, and thus, the disulfide, hydrogen, ionic bonds, and steric and hydrophobic interactions have to be broken down (Zhang et al. 2003). For this purpose, again, 1 M NaOH was added into the SPI solution and heat was applied. PVA and SPI solutions were mixed with a mass ratio of 50:50, so that a homogeneous solution was prepared. Triton X-100 at a ratio of 5 wt% on the basis of PVA mass was added into the final solution to reduce the surface tension of water and delay the gelation of PVA, since water as a solvent would lead to the formation of beads in the process of electrospinning. Again, 5 wt% of the glycerol on the basis of the final solution was added.
A 5 mL plastic syringe was loaded with the final solution to put in the electrospinning machine (Fanavaran Nano-Meghyas(. An 18-gauge needle was used and connected to the positive charge of the power supply. The voltage of 25 kV was applied and the distance between the tip of the needle and the collector was set to 15 cm. Speed of the rotatory collector was chosen to be 300 rpm. The solution was infused by amicropump toward the collector at a rate of 0.5 mL/h. This process was carried out at room temperature (Cho et al. 2010).
Since these constructs are made of hydrophilic-based materials, they need to be prevented from dissolution upon hydration. ENMs dissolved immediately after immersion in water, whereas it took time for CFs to be dissolved. Yet, CFs were susceptible to dissolution in water. Hence, GA was used as a cross-linker agent for immersion of the specimens in its solution.
In immersion method, 5% GA was diluted by acetone with the proportion of 10:90 (v/v) (10 refers to 5% GA and 90 refers to acetone). Since GA activates in an acidic environment, a sufficient amount of HCl was added to the solution to adjust the pH. CFs and ENMs were immersed in the solution of 5% GA/acetone (10:90 v/v) for 12 h and then were put in an oven at 50 °C for another 12 h. After that, to remove the unreacted GA, samples were washed in distilled water for 2 h on a shaker. Every hour, the distilled water was renewed with a fresh one (Qiu 2012).
Scanning electron microscopy (SEM)
To observe the morphology and microstructure of the CFs and ENMs, and cell adhesion, SEM (Seron Technologies Inc AIS2100) with the accelerating voltage of 15 kV was used.
Fourier transform infrared (FTIR) spectra analysis
FTIR spectra were obtained for SPI powder, PVA powder, CFs, and ENMs with and without glycerol, uncrosslinked and crosslinked PVA/SPI/glycerol CFs and ENMs. FTIR measurements were recorded in the range of 4000–400 cm−1 at a resolution of 4 cm−1 using 40 scans on the Nicolet Nexus spectrometer.
Water contact angle (WCA)
Water contact angle in the air on the surface of crosslinked CFs and ENMs was measured based on the ASTM D724-99 standard. The WCA was evaluated as the average value of measurements made on the opposite side of water drops (n = 5).
Simulated exudate solution uptake
Composition of the simulated wound exudate solutions
Simulated thin exudate (solution A)
1000 g water
0.368 g calcium chloride
8.298 g sodium chloride
Water vapor transmission rate (WVTR)
Specimens were prepared for tensile test. Samples were cut into a dog-bone shape of 1 × 6 cm for CFs and 1 × 3 cm for ENMs (n = 3). The sample’s thickness was measured prior its test using a micrometer with a sensitivity of 1 µm. The test was performed at room temperature using a cross-head speed of 5 mm/min for CFs and 1 mm/min for ENMs. The percentage of elongation-at-breakpoint and ultimate tensile strength (UTS) were determined by Instron 5566 tensile tester.
An ideal material must be non-toxic and biocompatible even its degraded products. Hence, the CFs and ENMs were evaluated to study the effect of these structures on living cells by the tests, as described below.
L929 mouse fibroblast cells were thawed and cultured in DMEM (Dulbecco’s Modified Eagle’s Medium) supplemented with 10% fetal bovine serum and 1% (v/v) penicillin–streptomycin. Cells were cultured in a humidified atmosphere of 5% CO2 at 37 °C in an incubator. When the cells reached the confluence of 70%, they were detached using trypsin enzyme and seeded into the 12-well plates.
To evaluate cell adhesion and morphology, crosslinked CFs and ENMs were sterilized. Both types of samples were washed in 70% ethanol twice and several times in phosphate buffer each for 15 min. After that, samples were immersed in culture medium for 12 h. 300 µL of cell suspension with the intensity of 105 cell/cm2 was added to the wells containing samples and medium (n = 3). They were kept in an incubator for 48 h; then, CFs and ENMs containing cells were prepared for observation of cell adhesion using SEM.
Excel software was used for statistical analysis. Comparison made between more than two groups was performed using ANOVA method. All errors and error bars present standard deviation (SD) from the mean. OriginPro version 9.3 was used to draw graphs. The contact angle and fiber diameter measurements of ENMs were carried out using Image J software and 100 fibers were chosen randomly to calculate the average fiber diameter.
Fourier transform infrared spectra (FTIR) analysis
In SPI powder, the amino acid group has a peak at 3300 cm−1 and stretching C–H band is vibrated at 2850 cm−1. By precisely looking at amid groups in SPI powder, the determined peaks at the range of 1700–1600 cm−1 refer to the stretching C=O of amid I band and peaks at the range of 1575–1480 cm−1 refer to the bending N–H of amid II. Peaks at the range of 1472–1241 attribute to the (C) O–O, stretching C–N band, bending N–H of amid III band, and the presence of β sheets in the structure of soy protein. The broadening peak at the range of 3500–3000 can be attributed to the free and connected N–H and O–H bands that enable the protein structure to form a hydrogen bond with the carbonyl group of peptide bond (Koshy et al. 2015; Ramji and Shah 2014; Su et al. 2010a, b).
Water contact angle (WCA)
One of the biocompatibility criteria of a biomaterial is surface hydrophilicity. Surface hydrophilicity is an important indicator of a proper cell-surface interaction which can be appraised by water contact angle test (Bahrami et al. 2019). Contact angle measurement is a good indicator of the CFs and ENMs hydrophilicity. No angle was formed on the surface of the ENMs. This can be attributed to the porous structure of the nanofibers that the drop of water penetrates into the construct; therefore, measuring the WCA was not possible and no angle was formed. Hence, due to increased porosity, the permeability of the samples against water droplets has increased. All the values for CFs were in the range of 0 ˂ θ ˂ 90, so they can be considered as hydrophilic. The contact angle value of the CFs was 72.79˚ ± 4.7.
Simulated exudate solution uptake
Water vapor transmission rate (WVTR)
The features of the CFs are attributed to the presence of glycerol and PVA in the structure, since the previous literature reported that pure SPI films were not flexible (Su et al. 2007). By comparing to the previous studies, the average fiber diameter decreased as glycerol was added (Cho et al. 2010). This result was expected in that by being positioned within the three-dimensional network of the protein by a plasticizer, the free volume will be increased and the mobility of the polymer chains will be easier (Koshy et al. 2015). Therefore, it would have an effect on the viscosity of the solution and simultaneously would have a direct effect on the fiber diameter.
FTIR spectrum of PVA confirmed the presence of all peaks related to hydroxyl and acetate groups. The spectrum of SPI presents the presence of amino acid proteins. The results of FTIR spectra showed the presence of amino acid proteins and glycerol in the bulk of CFs and ENMs. In addition, the spectrum confirmed the presence of GA in the structure of the specimens, so the crosslinking was successful.
Due to the porous structure of the ENMs, it was expected that their simulated exudate solution uptake percentage would be higher than CFs. The dense structure of the CFs did not allow for the water uptake. The greater amount of ENM’s water uptake makes it a suitable wound dressing for highly draining wounds and bleeding wounds. CFs and ENMs exhibited different stages of water uptake during the 48 h of immersion in the simulated exudate solution. There was an increasing uptake which is due to the influx of water into the specimens. The descending pattern in the water uptake is as the result of a spring-like contraction in the crosslinked network and secretion of glycerol molecules and water. The next escalations in the water uptake pattern after every decrease are because of the polymeric chain relaxation and a swollen matrix (Peles and Zilberman 2012).
The WVTR value of a normal skin is about 204 g m−2 day−1,and in severe burns, this value may reach 5138 g m−2 day−1(Peles and Zilberman 2012). The high WVTR value of ENMs is clearly due to the porous nature of the fibers that allows more evaporative water loss through itself. Indeed, the structural properties (thickness and porosity) would determine the diffusion of water through membranes and material’s hydrophilicity of the specimens would affect the WVTR values (Peles and Zilberman 2012). Keeping moisture in wound bed is crucial. CF’s low WVTR value would obstruct the wound healing due to poor drainage of the absorbed exudation.
It was reported that polyol-based plasticizers (compounds containing multiple hydroxyl groups) would reduce the mechanical strength and increase the flexibility when it forms hydrogen bonds and penetrates between protein chains (Peles and Zilberman 2012). In crosslinking using GA, aldehyde groups on both sides react with amino groups resulting in forming a network, and by this mean, it will increase the mechanical strength. The presence of glycerol may lead to an unwanted interaction between GA and glycerol itself; therefore, it may block the interaction between active aldehyde groups and amino groups of the protein resulting in a brittle behavior. Besides this, alcoholic nature of PVA and the presence of hydroxyl groups can also react with glycerol and may generate water as its side products; therefore, it may lead to a reduction in the activity of the cross-linker agent.
Both CF and ENM supported the cytocompatibility. It is known that topography of the surface plays an important role in the cell’s behavior. Nanostructure of the fibers would result in an increase in the surface area which would ease the accessibility of cells to absorb the serum protein (Fukushima 1969).
SEM experiments were performed in the Central Laboratory of Amirkabir University of Technology (Tehran Polytechnic). Thanks to Dr. Davoud Sadeghi and Mr. Masoud Dadras Chomachayi who provided help during the research.
- Fukushima D (1969) Denaturation of soybean proteins by organic solvents. Cereal Chem 46:156–163Google Scholar
- Khorshidi S, Solouk A, Karkhaneh A, Mirzadeh H, Sharifi S, Mazinani S (2016a) Effect of crosslinking procedure on structural, thermal, and functional performances of cellulosic nanofibers: a comparison between chemical and photochemical crosslinking. J Appl Polym Sci 133(34):1–9. https://doi.org/10.1002/app.43832 CrossRefGoogle Scholar
- Lovett J, Roberts S, Stephenson C (2006) Assessment of the uptake of simulated viscous exudate by adhesive foam dressings 15(4):2006Google Scholar
- Qiu K (2012) Biobased and biodegradable polymer nanocomposites. PhD dissertation. Cornell University. https://ecommons.cornell.edu/handle/1813/31221. Accessed 18 May 2018
- Shankar A, Seyam AM, Hudson SM (2013) Electrospinning of soy protein fibers and their compatibility with synthetic polymers. J Text Appar Technol Manag 8(1):1–14Google Scholar
- Su JF, Huang Z, Liu K, Ling Ling F, Liu HR (2007) Mechanical properties, biodegradation and water vapor permeability of blend films of soy protein isolate and poly (Vinyl Alcohol) compatibilized by glycerol. Polym Bull 58(5–6):913–921. https://doi.org/10.1007/s00289-007-0731-7 CrossRefGoogle Scholar
- Su JF, Yuan XY, Huang Z, Xia WL (2010b) Properties stability and biodegradation behaviors of soy protein isolate/poly (Vinyl Alcohol) blend films. Polym Degrad Stab 95(7):1226–1237. https://doi.org/10.1016/j.polymdegradstab.2010.03.035 CrossRefGoogle Scholar
Open AccessThis article is distributed under the terms of the Creative Commons Attribution 4.0 International License (http://creativecommons.org/licenses/by/4.0/), which permits unrestricted use, distribution, and reproduction in any medium, provided you give appropriate credit to the original author(s) and the source, provide a link to the Creative Commons license, and indicate if changes were made.